#------------------------------------------------------------------------------
#$Date: 2023-12-08 16:16:31 +0200 (Fri, 08 Dec 2023) $
#$Revision: 288183 $
#$URL: file:///home/coder/svn-repositories/cod/cif/4/31/32/4313240.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4313240
loop_
_publ_author_name
'Shahrad Amerioun'
'Sergei I. Simak'
'Ulrich Häussermann'
_publ_section_title
;
 Laves-Phase Structural Changes in the System CaAl2-xMgx
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              1467
_journal_page_last               1474
_journal_paper_doi               10.1021/ic020596m
_journal_volume                  42
_journal_year                    2003
_chemical_formula_sum            'Al0.93 Ca Mg1.07'
_chemical_formula_weight         91.2
_space_group_IT_number           194
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  '-P 6c 2c'
_symmetry_space_group_name_H-M   'P 63/m m c'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            8
_cell_length_a                   5.935(1)
_cell_length_b                   5.935(1)
_cell_length_c                   19.258(6)
_cell_measurement_reflns_used    29
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      43.4
_cell_measurement_theta_min      14.5
_cell_volume                     587.5(2)
_computing_cell_refinement       'PIRUM (Werner & Ericsson, 1993)'
_computing_data_collection       'EXPOSE in IPDS (Stoe & Cie, 1997)'
_computing_data_reduction        'X-RED  (Stoe & Cie, 1997)'
_computing_molecular_graphics    'Atoms (Dowty, 1997)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_detector_area_resol_mean 'area detector'
_diffrn_measured_fraction_theta_full 0.991
_diffrn_measured_fraction_theta_max 0.991
_diffrn_measurement_device_type  'Stoe IPDS (version 2.87)'
_diffrn_measurement_method       'f scan'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0892
_diffrn_reflns_av_sigmaI/netI    0.0269
_diffrn_reflns_limit_h_max       7
_diffrn_reflns_limit_h_min       -6
_diffrn_reflns_limit_k_max       7
_diffrn_reflns_limit_k_min       -7
_diffrn_reflns_limit_l_max       25
_diffrn_reflns_limit_l_min       -25
_diffrn_reflns_number            4983
_diffrn_reflns_theta_full        28.12
_diffrn_reflns_theta_max         28.12
_diffrn_reflns_theta_min         3.96
_diffrn_standards_number         6.0
_exptl_absorpt_coefficient_mu    2.281
_exptl_absorpt_correction_T_max  0.7280
_exptl_absorpt_correction_T_min  0.6717
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_process_details   'X-shape, (Stoe & Cie, 1997)'
_exptl_crystal_colour            Silver
_exptl_crystal_density_diffrn    2.055
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       'irregular shape'
_exptl_crystal_F_000             360
_exptl_crystal_size_max          0.02
_exptl_crystal_size_mid          0.02
_exptl_crystal_size_min          0.015
_refine_diff_density_max         1.427
_refine_diff_density_min         -1.341
_refine_diff_density_rms         0.245
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.881
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     18
_refine_ls_number_reflns         318
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.881
_refine_ls_R_factor_all          0.0497
_refine_ls_R_factor_gt           0.0184
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0000P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0175
_refine_ls_wR_factor_ref         0.0321
_reflns_number_gt                191
_reflns_number_total             318
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic020596m_3.cif
_cod_data_source_block           CaAl0.93Mg1.07
_cod_depositor_comments
;
The following automatic conversions were performed:

data name '_atom_site_symetry_multiplicity' was replaced with
'_atom_site_symmetry_multiplicity' as specified in the replacement
file 'data/replacement-values/replacement_tags.lst'.

Automatic conversion script
Id: cif_correct_tags 9268 2022-04-12 08:56:07Z antanas 
;
_cod_original_formula_sum        CaAl0.93Mg1.07
_cod_database_code               4313240
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'-x, -y, z+1/2'
'y, -x+y, z+1/2'
'x-y, x, z+1/2'
'y, x, -z'
'x-y, -y, -z'
'-x, -x+y, -z'
'-y, -x, -z+1/2'
'-x+y, y, -z+1/2'
'x, x-y, -z+1/2'
'-x, -y, -z'
'y, -x+y, -z'
'x-y, x, -z'
'x, y, -z-1/2'
'-y, x-y, -z-1/2'
'-x+y, -x, -z-1/2'
'-y, -x, z'
'-x+y, y, z'
'x, x-y, z'
'y, x, z-1/2'
'x-y, -y, z-1/2'
'-x, -x+y, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Ca1 Ca 0.3333 0.6667 0.34313(5) 0.0116(2) Uani 1 6 d S . .
Ca2 Ca 0.0000 0.0000 0.40560(5) 0.0120(3) Uani 1 6 d S . .
AL1 Mg 0.3267(3) 0.16336(15) 0.2500 0.0076(3) Uani 1 4 d S . .
Al2 Al 0.3333 0.6667 0.62854(7) 0.0149(3) Uani 1 6 d S . .
MG1 Al 0.0000 0.5000 0.5000 0.0159(3) Uani 1 4 d S . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Ca Ca 0.2262 0.3064 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mg Mg 0.0486 0.0363 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Al Al 0.0645 0.0514 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
AL1 Ca1 AL1 51.73(5) 2 3_565 ?
AL1 Ca1 AL1 95.63(2) 2 1_565 ?
AL1 Ca1 AL1 49.58(5) 3_565 1_565 ?
AL1 Ca1 AL1 117.65(3) 2 2_665 ?
AL1 Ca1 AL1 95.63(2) 3_565 2_665 ?
AL1 Ca1 AL1 51.73(5) 1_565 2_665 ?
AL1 Ca1 AL1 49.58(5) 2 . ?
AL1 Ca1 AL1 95.63(2) 3_565 . ?
AL1 Ca1 AL1 117.65(3) 1_565 . ?
AL1 Ca1 AL1 95.63(2) 2_665 . ?
AL1 Ca1 AL1 95.63(2) 2 3_665 ?
AL1 Ca1 AL1 117.65(3) 3_565 3_665 ?
AL1 Ca1 AL1 95.63(2) 1_565 3_665 ?
AL1 Ca1 AL1 49.58(5) 2_665 3_665 ?
AL1 Ca1 AL1 51.73(5) . 3_665 ?
AL1 Ca1 Al2 144.89(3) 2 13_676 ?
AL1 Ca1 Al2 94.12(3) 3_565 13_676 ?
AL1 Ca1 Al2 49.80(3) 1_565 13_676 ?
AL1 Ca1 Al2 49.80(3) 2_665 13_676 ?
AL1 Ca1 Al2 144.89(3) . 13_676 ?
AL1 Ca1 Al2 94.12(3) 3_665 13_676 ?
AL1 Ca1 Al2 49.80(3) 2 13_566 ?
AL1 Ca1 Al2 49.80(3) 3_565 13_566 ?
AL1 Ca1 Al2 94.12(3) 1_565 13_566 ?
AL1 Ca1 Al2 144.89(3) 2_665 13_566 ?
AL1 Ca1 Al2 94.12(3) . 13_566 ?
AL1 Ca1 Al2 144.89(3) 3_665 13_566 ?
Al2 Ca1 Al2 117.571(15) 13_676 13_566 ?
AL1 Ca1 Al2 94.12(3) 2 13_666 ?
AL1 Ca1 Al2 144.89(3) 3_565 13_666 ?
AL1 Ca1 Al2 144.89(3) 1_565 13_666 ?
AL1 Ca1 Al2 94.12(3) 2_665 13_666 ?
AL1 Ca1 Al2 49.80(3) . 13_666 ?
AL1 Ca1 Al2 49.80(3) 3_665 13_666 ?
Al2 Ca1 Al2 117.571(16) 13_676 13_666 ?
Al2 Ca1 Al2 117.571(16) 13_566 13_666 ?
AL1 Ca1 MG1 144.88(2) 2 3_565 ?
AL1 Ca1 MG1 116.454(18) 3_565 3_565 ?
AL1 Ca1 MG1 95.019(15) 1_565 3_565 ?
AL1 Ca1 MG1 95.019(15) 2_665 3_565 ?
AL1 Ca1 MG1 144.88(2) . 3_565 ?
AL1 Ca1 MG1 116.454(19) 3_665 3_565 ?
Al2 Ca1 MG1 51.41(3) 13_676 3_565 ?
Al2 Ca1 MG1 96.11(3) 13_566 3_565 ?
Al2 Ca1 MG1 96.11(3) 13_666 3_565 ?
AL1 Ca1 MG1 95.019(15) 2 . ?
AL1 Ca1 MG1 95.019(15) 3_565 . ?
AL1 Ca1 MG1 116.454(19) 1_565 . ?
AL1 Ca1 MG1 144.88(2) 2_665 . ?
AL1 Ca1 MG1 116.454(19) . . ?
AL1 Ca1 MG1 144.88(2) 3_665 . ?
Al2 Ca1 MG1 96.11(3) 13_676 . ?
Al2 Ca1 MG1 51.41(2) 13_566 . ?
Al2 Ca1 MG1 96.11(3) 13_666 . ?
MG1 Ca1 MG1 50.543(17) 3_565 . ?
AL1 Ca1 MG1 116.454(18) 2 2_665 ?
AL1 Ca1 MG1 144.88(2) 3_565 2_665 ?
AL1 Ca1 MG1 144.88(2) 1_565 2_665 ?
AL1 Ca1 MG1 116.454(19) 2_665 2_665 ?
AL1 Ca1 MG1 95.019(15) . 2_665 ?
AL1 Ca1 MG1 95.019(15) 3_665 2_665 ?
Al2 Ca1 MG1 96.11(3) 13_676 2_665 ?
Al2 Ca1 MG1 96.11(3) 13_566 2_665 ?
Al2 Ca1 MG1 51.41(2) 13_666 2_665 ?
MG1 Ca1 MG1 50.543(17) 3_565 2_665 ?
MG1 Ca1 MG1 50.543(17) . 2_665 ?
AL1 Ca2 AL1 50.06(4) 3 2 ?
AL1 Ca2 AL1 50.06(4) 3 . ?
AL1 Ca2 AL1 50.06(4) 2 . ?
AL1 Ca2 MG1 144.77(2) 3 2_665 ?
AL1 Ca2 MG1 117.138(14) 2 2_665 ?
AL1 Ca2 MG1 95.48(3) . 2_665 ?
AL1 Ca2 MG1 117.138(14) 3 3 ?
AL1 Ca2 MG1 144.77(2) 2 3 ?
AL1 Ca2 MG1 95.48(2) . 3 ?
MG1 Ca2 MG1 50.458(9) 2_665 3 ?
AL1 Ca2 MG1 144.77(2) 3 . ?
AL1 Ca2 MG1 95.48(3) 2 . ?
AL1 Ca2 MG1 117.138(14) . . ?
MG1 Ca2 MG1 50.458(9) 2_665 . ?
MG1 Ca2 MG1 95.17(2) 3 . ?
AL1 Ca2 MG1 95.48(3) 3 2 ?
AL1 Ca2 MG1 117.138(14) 2 2 ?
AL1 Ca2 MG1 144.77(2) . 2 ?
MG1 Ca2 MG1 116.96(3) 2_665 2 ?
MG1 Ca2 MG1 95.17(2) 3 2 ?
MG1 Ca2 MG1 95.17(2) . 2 ?
AL1 Ca2 MG1 117.138(14) 3 3_455 ?
AL1 Ca2 MG1 95.48(3) 2 3_455 ?
AL1 Ca2 MG1 144.77(2) . 3_455 ?
MG1 Ca2 MG1 95.17(2) 2_665 3_455 ?
MG1 Ca2 MG1 116.96(3) 3 3_455 ?
MG1 Ca2 MG1 50.458(9) . 3_455 ?
MG1 Ca2 MG1 50.458(9) 2 3_455 ?
AL1 Ca2 MG1 95.48(2) 3 1_545 ?
AL1 Ca2 MG1 144.77(2) 2 1_545 ?
AL1 Ca2 MG1 117.138(14) . 1_545 ?
MG1 Ca2 MG1 95.17(2) 2_665 1_545 ?
MG1 Ca2 MG1 50.458(9) 3 1_545 ?
MG1 Ca2 MG1 116.96(3) . 1_545 ?
MG1 Ca2 MG1 50.458(9) 2 1_545 ?
MG1 Ca2 MG1 95.17(2) 3_455 1_545 ?
AL1 Ca2 Al2 94.32(3) 3 13_566 ?
AL1 Ca2 Al2 49.88(3) 2 13_566 ?
AL1 Ca2 Al2 94.32(3) . 13_566 ?
MG1 Ca2 Al2 95.658(15) 2_665 13_566 ?
MG1 Ca2 Al2 145.45(3) 3 13_566 ?
MG1 Ca2 Al2 51.21(2) . 13_566 ?
MG1 Ca2 Al2 95.658(15) 2 13_566 ?
MG1 Ca2 Al2 51.21(2) 3_455 13_566 ?
MG1 Ca2 Al2 145.45(3) 1_545 13_566 ?
AL1 Ca2 Al2 49.88(3) 3 13_556 ?
AL1 Ca2 Al2 94.32(3) 2 13_556 ?
AL1 Ca2 Al2 94.32(3) . 13_556 ?
MG1 Ca2 Al2 145.45(3) 2_665 13_556 ?
MG1 Ca2 Al2 95.658(14) 3 13_556 ?
MG1 Ca2 Al2 145.45(3) . 13_556 ?
MG1 Ca2 Al2 51.21(2) 2 13_556 ?
MG1 Ca2 Al2 95.658(15) 3_455 13_556 ?
MG1 Ca2 Al2 51.21(2) 1_545 13_556 ?
Al2 Ca2 Al2 116.528(19) 13_566 13_556 ?
AL1 Ca2 Al2 94.32(3) 3 13_666 ?
AL1 Ca2 Al2 94.32(3) 2 13_666 ?
AL1 Ca2 Al2 49.88(3) . 13_666 ?
MG1 Ca2 Al2 51.21(2) 2_665 13_666 ?
MG1 Ca2 Al2 51.21(2) 3 13_666 ?
MG1 Ca2 Al2 95.658(15) . 13_666 ?
MG1 Ca2 Al2 145.45(3) 2 13_666 ?
MG1 Ca2 Al2 145.45(3) 3_455 13_666 ?
MG1 Ca2 Al2 95.658(15) 1_545 13_666 ?
Al2 Ca2 Al2 116.528(19) 13_566 13_666 ?
Al2 Ca2 Al2 116.528(19) 13_556 13_666 ?
AL1 AL1 AL1 60.0 3 2 ?
AL1 AL1 Al2 121.20(2) 3 13_666 ?
AL1 AL1 Al2 121.20(2) 2 13_666 ?
AL1 AL1 Al2 121.20(2) 3 4_664 ?
AL1 AL1 Al2 121.20(2) 2 4_664 ?
Al2 AL1 Al2 106.53(6) 13_666 4_664 ?
AL1 AL1 AL1 180.0 3 3_665 ?
AL1 AL1 AL1 120.0 2 3_665 ?
Al2 AL1 AL1 58.80(2) 13_666 3_665 ?
Al2 AL1 AL1 58.80(2) 4_664 3_665 ?
AL1 AL1 AL1 120.0 3 2_655 ?
AL1 AL1 AL1 180.00(6) 2 2_655 ?
Al2 AL1 AL1 58.80(2) 13_666 2_655 ?
Al2 AL1 AL1 58.80(2) 4_664 2_655 ?
AL1 AL1 AL1 60.0 3_665 2_655 ?
AL1 AL1 Ca2 64.97(2) 3 16_556 ?
AL1 AL1 Ca2 64.97(2) 2 16_556 ?
Al2 AL1 Ca2 172.51(5) 13_666 16_556 ?
Al2 AL1 Ca2 65.98(2) 4_664 16_556 ?
AL1 AL1 Ca2 115.03(2) 3_665 16_556 ?
AL1 AL1 Ca2 115.03(2) 2_655 16_556 ?
AL1 AL1 Ca2 64.97(2) 3 . ?
AL1 AL1 Ca2 64.97(2) 2 . ?
Al2 AL1 Ca2 65.98(2) 13_666 . ?
Al2 AL1 Ca2 172.51(5) 4_664 . ?
AL1 AL1 Ca2 115.03(2) 3_665 . ?
AL1 AL1 Ca2 115.03(2) 2_655 . ?
Ca2 AL1 Ca2 121.51(5) 16_556 . ?
AL1 AL1 Ca1 65.21(2) 3 16_546 ?
AL1 AL1 Ca1 115.87(2) 2 16_546 ?
Al2 AL1 Ca1 114.14(3) 13_666 16_546 ?
Al2 AL1 Ca1 65.124(15) 4_664 16_546 ?
AL1 AL1 Ca1 114.79(2) 3_665 16_546 ?
AL1 AL1 Ca1 64.13(2) 2_655 16_546 ?
Ca2 AL1 Ca1 63.460(16) 16_556 16_546 ?
Ca2 AL1 Ca1 117.15(2) . 16_546 ?
AL1 AL1 Ca1 65.21(2) 3 1_545 ?
AL1 AL1 Ca1 115.87(2) 2 1_545 ?
Al2 AL1 Ca1 65.124(15) 13_666 1_545 ?
Al2 AL1 Ca1 114.14(3) 4_664 1_545 ?
AL1 AL1 Ca1 114.79(2) 3_665 1_545 ?
AL1 AL1 Ca1 64.13(2) 2_655 1_545 ?
Ca2 AL1 Ca1 117.15(2) 16_556 1_545 ?
Ca2 AL1 Ca1 63.460(16) . 1_545 ?
Ca1 AL1 Ca1 62.34(3) 16_546 1_545 ?
AL1 AL1 Ca1 115.87(2) 3 . ?
AL1 AL1 Ca1 65.21(2) 2 . ?
Al2 AL1 Ca1 65.124(15) 13_666 . ?
Al2 AL1 Ca1 114.14(3) 4_664 . ?
AL1 AL1 Ca1 64.13(2) 3_665 . ?
AL1 AL1 Ca1 114.79(2) 2_655 . ?
Ca2 AL1 Ca1 117.15(2) 16_556 . ?
Ca2 AL1 Ca1 63.460(16) . . ?
Ca1 AL1 Ca1 178.88(5) 16_546 . ?
Ca1 AL1 Ca1 117.65(3) 1_545 . ?
AL1 AL1 Ca1 115.87(2) 3 16_556 ?
AL1 AL1 Ca1 65.21(2) 2 16_556 ?
Al2 AL1 Ca1 114.14(3) 13_666 16_556 ?
Al2 AL1 Ca1 65.124(15) 4_664 16_556 ?
AL1 AL1 Ca1 64.13(2) 3_665 16_556 ?
AL1 AL1 Ca1 114.79(2) 2_655 16_556 ?
Ca2 AL1 Ca1 63.460(16) 16_556 16_556 ?
Ca2 AL1 Ca1 117.15(2) . 16_556 ?
Ca1 AL1 Ca1 117.65(3) 16_546 16_556 ?
Ca1 AL1 Ca1 178.88(5) 1_545 16_556 ?
Ca1 AL1 Ca1 62.34(3) . 16_556 ?
AL1 Al2 AL1 62.39(5) 14_566 13_666 ?
AL1 Al2 AL1 62.39(5) 14_566 15_556 ?
AL1 Al2 AL1 62.39(5) 13_666 15_556 ?
AL1 Al2 Ca1 65.07(2) 14_566 13_676 ?
AL1 Al2 Ca1 65.07(2) 13_666 13_676 ?
AL1 Al2 Ca1 117.68(5) 15_556 13_676 ?
AL1 Al2 Ca1 65.07(2) 14_566 13_566 ?
AL1 Al2 Ca1 117.68(5) 13_666 13_566 ?
AL1 Al2 Ca1 65.07(2) 15_556 13_566 ?
Ca1 Al2 Ca1 117.571(15) 13_676 13_566 ?
AL1 Al2 Ca1 117.68(5) 14_566 13_666 ?
AL1 Al2 Ca1 65.07(2) 13_666 13_666 ?
AL1 Al2 Ca1 65.07(2) 15_556 13_666 ?
Ca1 Al2 Ca1 117.571(16) 13_676 13_666 ?
Ca1 Al2 Ca1 117.571(16) 13_566 13_666 ?
AL1 Al2 Ca2 64.14(3) 14_566 13_566 ?
AL1 Al2 Ca2 116.41(3) 13_666 13_566 ?
AL1 Al2 Ca2 116.41(3) 15_556 13_566 ?
Ca1 Al2 Ca2 62.921(5) 13_676 13_566 ?
Ca1 Al2 Ca2 62.921(5) 13_566 13_566 ?
Ca1 Al2 Ca2 178.18(6) 13_666 13_566 ?
AL1 Al2 Ca2 116.41(3) 14_566 13_556 ?
AL1 Al2 Ca2 116.41(3) 13_666 13_556 ?
AL1 Al2 Ca2 64.14(3) 15_556 13_556 ?
Ca1 Al2 Ca2 178.18(6) 13_676 13_556 ?
Ca1 Al2 Ca2 62.921(5) 13_566 13_556 ?
Ca1 Al2 Ca2 62.921(5) 13_666 13_556 ?
Ca2 Al2 Ca2 116.528(19) 13_566 13_556 ?
AL1 Al2 Ca2 116.41(3) 14_566 13_666 ?
AL1 Al2 Ca2 64.14(3) 13_666 13_666 ?
AL1 Al2 Ca2 116.41(3) 15_556 13_666 ?
Ca1 Al2 Ca2 62.921(5) 13_676 13_666 ?
Ca1 Al2 Ca2 178.18(6) 13_566 13_666 ?
Ca1 Al2 Ca2 62.921(5) 13_666 13_666 ?
Ca2 Al2 Ca2 116.528(19) 13_566 13_666 ?
Ca2 Al2 Ca2 116.528(19) 13_556 13_666 ?
MG1 MG1 MG1 180.0 3_565 3_455 ?
MG1 MG1 MG1 60.0 3_565 2_665 ?
MG1 MG1 MG1 120.0 3_455 2_665 ?
MG1 MG1 MG1 120.0 3_565 2_565 ?
MG1 MG1 MG1 60.0 3_455 2_565 ?
MG1 MG1 MG1 180.0 2_665 2_565 ?
MG1 MG1 Ca1 64.729(8) 3_565 . ?
MG1 MG1 Ca1 115.271(8) 3_455 . ?
MG1 MG1 Ca1 64.729(8) 2_665 . ?
MG1 MG1 Ca1 115.271(8) 2_565 . ?
MG1 MG1 Ca1 115.271(8) 3_565 13_566 ?
MG1 MG1 Ca1 64.729(8) 3_455 13_566 ?
MG1 MG1 Ca1 115.271(8) 2_665 13_566 ?
MG1 MG1 Ca1 64.729(8) 2_565 13_566 ?
Ca1 MG1 Ca1 180.0 . 13_566 ?
MG1 MG1 Ca2 64.771(4) 3_565 13_566 ?
MG1 MG1 Ca2 115.229(4) 3_455 13_566 ?
MG1 MG1 Ca2 115.229(4) 2_665 13_566 ?
MG1 MG1 Ca2 64.771(4) 2_565 13_566 ?
Ca1 MG1 Ca2 117.055(14) . 13_566 ?
Ca1 MG1 Ca2 62.945(14) 13_566 13_566 ?
MG1 MG1 Ca2 115.229(4) 3_565 . ?
MG1 MG1 Ca2 64.771(4) 3_455 . ?
MG1 MG1 Ca2 64.771(4) 2_665 . ?
MG1 MG1 Ca2 115.229(4) 2_565 . ?
Ca1 MG1 Ca2 62.945(14) . . ?
Ca1 MG1 Ca2 117.055(14) 13_566 . ?
Ca2 MG1 Ca2 180.0 13_566 . ?
MG1 MG1 Ca2 115.229(4) 3_565 13_556 ?
MG1 MG1 Ca2 64.771(4) 3_455 13_556 ?
MG1 MG1 Ca2 64.771(4) 2_665 13_556 ?
MG1 MG1 Ca2 115.229(4) 2_565 13_556 ?
Ca1 MG1 Ca2 117.055(14) . 13_556 ?
Ca1 MG1 Ca2 62.945(14) 13_566 13_556 ?
Ca2 MG1 Ca2 116.96(3) 13_566 13_556 ?
Ca2 MG1 Ca2 63.04(3) . 13_556 ?
MG1 MG1 Ca2 64.771(4) 3_565 1_565 ?
MG1 MG1 Ca2 115.229(4) 3_455 1_565 ?
MG1 MG1 Ca2 115.229(4) 2_665 1_565 ?
MG1 MG1 Ca2 64.771(4) 2_565 1_565 ?
Ca1 MG1 Ca2 62.945(14) . 1_565 ?
Ca1 MG1 Ca2 117.055(14) 13_566 1_565 ?
Ca2 MG1 Ca2 63.04(3) 13_566 1_565 ?
Ca2 MG1 Ca2 116.96(3) . 1_565 ?
Ca2 MG1 Ca2 180.0 13_556 1_565 ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Ca1 AL1 3.4737(6) 2 ?
Ca1 AL1 3.4737(6) 3_565 ?
Ca1 AL1 3.4737(6) 1_565 ?
Ca1 AL1 3.4737(6) 2_665 ?
Ca1 AL1 3.4737(6) . ?
Ca1 AL1 3.4737(7) 3_665 ?
Ca1 Al2 3.4751(6) 13_676 ?
Ca1 Al2 3.4751(6) 13_566 ?
Ca1 Al2 3.4751(6) 13_666 ?
Ca1 MG1 3.4809(10) 3_565 ?
Ca1 MG1 3.4809(10) . ?
Ca1 MG1 3.4809(10) 2_665 ?
Ca2 AL1 3.4427(13) 3 ?
Ca2 AL1 3.4427(13) 2 ?
Ca2 AL1 3.4427(13) . ?
Ca2 MG1 3.4864(7) 2_665 ?
Ca2 MG1 3.4864(7) 3 ?
Ca2 MG1 3.4864(7) . ?
Ca2 MG1 3.4864(7) 2 ?
Ca2 MG1 3.4864(7) 3_455 ?
Ca2 MG1 3.4864(7) 1_545 ?
Ca2 Al2 3.4945(6) 13_566 ?
Ca2 Al2 3.4945(6) 13_556 ?
Ca2 Al2 3.4945(6) 13_666 ?
AL1 AL1 2.913(3) 3 ?
AL1 AL1 2.913(3) 2 ?
AL1 Al2 2.9258(15) 13_666 ?
AL1 Al2 2.9258(15) 4_664 ?
AL1 AL1 3.031(3) 3_665 ?
AL1 AL1 3.031(3) 2_655 ?
AL1 Ca2 3.4427(13) 16_556 ?
AL1 Ca1 3.4737(6) 16_546 ?
AL1 Ca1 3.4737(6) 1_545 ?
AL1 Ca1 3.4737(7) 16_556 ?
Al2 AL1 2.9258(15) 14_566 ?
Al2 AL1 2.9258(15) 13_666 ?
Al2 AL1 2.9258(15) 15_556 ?
Al2 Ca1 3.4751(6) 13_676 ?
Al2 Ca1 3.4751(6) 13_566 ?
Al2 Ca1 3.4751(6) 13_666 ?
Al2 Ca2 3.4945(6) 13_566 ?
Al2 Ca2 3.4945(6) 13_556 ?
Al2 Ca2 3.4945(6) 13_666 ?
MG1 MG1 2.9721(4) 3_565 ?
MG1 MG1 2.9721(4) 3_455 ?
MG1 MG1 2.9721(5) 2_665 ?
MG1 MG1 2.9721(4) 2_565 ?
MG1 Ca1 3.4809(10) 13_566 ?
MG1 Ca2 3.4864(7) 13_566 ?
MG1 Ca2 3.4864(7) 13_556 ?
MG1 Ca2 3.4864(7) 1_565 ?
